Achieving Colour Tuneable and White-Light Luminescence in a Large Family of Dual-Emission Lanthanide Coordination Polymers
Qian, Junfeng; Lu, Huangjie; Zheng, Zhaofa; Xu, Miaomiao; Qian, Yuan; Zhang, Zhi-Hui; Wang, Jian-Qiang; He, Mingyang; Lin, Jian; Dalton Transactions  (2021) –; doi:10.1039/D1DT01618K

data_7708221
_publ_section_title
;
 Achieving Colour Tuneable and White-Light Luminescence in a Large Family
 of Dual-Emission Lanthanide Coordination Polymers
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D1DT01618K
_journal_year                    2021
_chemical_formula_moiety         'C18 N3 O6 Yb'
_chemical_formula_sum            'C18 N3 O6 Yb'
_chemical_formula_weight         527.25
_chemical_melting_point          ?
_chemical_name_common
'Ytterbium 2,2':6',2''-terpyridine-4'-carboxyli'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2021-07-16 deposited with the CCDC.	2021-09-06 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 124.353(4)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.945(2)
_cell_length_b                   9.4044(10)
_cell_length_c                   11.9566(14)
_cell_measurement_reflns_used    7383
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      55.002
_cell_measurement_theta_min      5.131
_cell_volume                     1665.9(3)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX3'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0409
_diffrn_reflns_av_unetI/netI     0.0267
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            10992
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.522
_diffrn_reflns_theta_min         2.565
_exptl_absorpt_coefficient_mu    5.657
_exptl_absorpt_correction_T_max  0.636
_exptl_absorpt_correction_T_min  0.512
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SHELTXPREP
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.102
_exptl_crystal_description       block
_exptl_crystal_F_000             988
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.08
_refine_diff_density_max         2.222
_refine_diff_density_min         -1.128
_refine_diff_density_rms         0.155
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.097
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     129
_refine_ls_number_reflns         1911
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.097
_refine_ls_R_factor_all          0.0329
_refine_ls_R_factor_gt           0.0299
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0512P)^2^+5.1436P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0801
_refine_ls_wR_factor_ref         0.0828
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1796
_reflns_number_total             1911
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d1dt01618k2.cif
_cod_data_source_block           YbTPC2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_chemical_melting_point' value 'N/a' was changed to '?' --
the value is undefined or not given.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_original_cell_volume        1665.8(3)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7708221
_shelxl_version_number           2014-3
_shelx_res_checksum              53814
_shelx_hkl_checksum              91081